Magnetic Fe doped ZnO nanofibers obtained by electrospinning
- 1.7k Downloads
We demonstrate structural and room temperature magnetic properties of Fe doped ZnO nanofibers (NFs) obtained by electrospinning followed by calcination. The observed NFs, formed from crystalographically oriented, approximately 4.5 nm particles conglomerates, were approximately 200 nm in diameter. The reported synthesis of room temperature ferromagnetic Fe doped ZnO NFs is both facile and economical, and is therefore suggested as a generic method of fabricating biocompatible magnetic materials. The major substrates selected for the NFs synthesis (Zn, Fe) comprised of relatively low toxicity materials. Incorporating 10% Fe into ZnO does not modify the wurtzite crystal structure of the host material. No evidence of impurity phase was detected by either X-ray or electron diffraction. Magnetometry studies and Magnetic Force Microscopy imaging reveal a local ferromagnetic order that persists up to room temperature. We suggest that the observed phenomenon is either due to a mechanism mediated by presence of oxygen vacancies and/or is related to iron-rich precipitates.
KeywordsElectrospinning ZnO nanofibers ZnFeO Room temperature ferromagnetism Magnetic oxides
The physical origin and the occurrence of ZnO doped with transition metal cations ferromagnetism are subject to active research. In spite of numerous studies the ferromagnetic properties of transition metal cations doped wurtzite ZnO host is still a controversial issue [1, 2, 3, 4, 5, 6]. A high temperature ferromagnetism was reported numerously for Co doped ZnO in thin films produced by all accessible methods including pulsed layer deposition , the magnetron co-sputtering , the sol–gel method , and epitaxial thin films . Recently, Fe doped ZnO nanostructures, synthesized by the sol–gel method, were observed to be ferromagnetic . The observed room temperature ferromagnetism was reported to be an intrinsic Fe doped ZnO property. Interestingly, neither Fe, nor FeO and Fe2O3 phase in the Fe doped ZnO nanoparticles were observed based on X-ray absorption near edge structure measurements . On the other hand, there are report claiming no essential role of the transition metals in the ZnO magnetism in low dimension Fe and Mn doped ZnO films . In particular, based on the magnetic properties of Mn doped ZnO layers, after subtraction of the substrate effects, no evidence of a sample ferromagnetism was observed . Both reports point that a significant contribution to the room temperature ferromagnetism comes from the surface and/or the interface defects located between the sample and substrate. Interestingly, ferromagnetism has been also reported in thin films and nanoparticles of a large family of undoped wide gap semiconductors (ZnO, TiO2, HfO2, SnO2, etc.) . The ferromagnetism observed in the semiconductor nanostructures was attributed to oxygen defects which are of special significance in low dimension samples . Additionally, based on a study of laser-deposited thin films of Zn1−xCoxO, the antiferromagnetic super exchange interaction was proposed to be the dominant mechanism for the exchange coupling between Co and Zn1−xCoxO . Similar explanation was provided for polycrystalline powders synthesized by two different methods: solid-state and liquid-phase reactions . The above observations have their foundation in calculations of the local spin density functional theory for Zn1−xCox . The authors observed that the dominant magnetic interaction in well-characterized stochiometric phase (x up to 0.15) is dominated by the near neighbour antiferromagnetic coupling and these calculations suggested that ferromagnetism will only occur in the presence of additional hole doping. Based on similar calculations a short range nature of ferromagnetic and antiferromagnetic interactions was observed and a spin-glass like state was noted based on energy considerations for Co doped ZnO . Recently, defect induced Fe doped ZnO reversible ferromagnetism was reported and attributed to hydrogen mediated oxygen vacancies . Similarly, ferromagnetic Co doped ZnO was reported and reversible manipulation of short-range spin ordering by injection and ejection of hydrogen was demonstrated .
1D semiconductor nanostructures such as wires, tubes, belts and fibers have attracted a great deal of attention in recent years. Among many techniques, which allow to obtain 1D semiconductors, electrospinning is one of the most simple, versatile, low-cost, and effective. The method has an attractive potential for producing NFs from polymers, composites or ceramics with diameters ranging from tens of nanometers to microns [20, 21, 22, 23, 24]. Moreover, NFs length is limited only by the stability of process parameters, time, and amount of applied material [23, 24]. In particular, electrospinning, followed by calcination, is a versatile way to synthesize ZnO nanofibers [25, 26, 27]. The nanofibers consist of conglomerates of nanostructured polycrystalline domains, which are responsible for their very large surface to volume ratio. ZnO doped with transition metal ions such as Co, Mn, Ni or Fe is a promising candidate for a room temperature ferromagnetic semiconductor . Additionally, combining the ability to form NFs with transition metal doping makes the electrospinning a very promising method for providing magnetic nanofibers with potential applications in magnetic sensors, flexible magnets and biosensors.
In this study, we demonstrate the feasibility of obtaining Fe doped ZnO nanofibers exhibiting ferromagnetism above room temperature. We show that the ferromagnetic signal derives from a collective behavior typical for a blocked super paramagnet and estimate the size of nano crystallites which form the blocked state. We point out that incorporating 10% Fe into ZnO in electrospun materials does not lead to sizeable precipitates of other impurity phases and discuss possible origins of the ferromagnetic coupling. The synthesized material is non toxic thus could have potential biomedical applications [29, 30, 31].
2.1 Electrospinning and calcinations
We prepared undoped and iron doped ZnO nanofibers by a procedure, which consisted of four steps. The first step was to obtain 10% (wt) solution of poly(vinyl alcohol) (PVA, MW = 72,000) (C2H4)n (POCH, Poland) in deionized water (0.08 μS). Aqueous solution of PVA was prepared by keeping the mixture at 60 °C for 7 days. The second step was a sol–gel process, 0.25 g of zinc acetate dihydrate (Zn(CH3COO)2·2H2O) (CHEMPUR, Poland) was dissolved in 1.25 g solution of PVA as a precursor to obtain ZnO nanofibers. Fe doping was realized by adding 0.022 g iron acetate (CH3CO2)2Fe (Sigma Aldrich) to the mixture. The atomic ratio of Fe to Zn ions was about 0.1. The following step was the electrospinning process. The flow rate was stabilized at 0.2 ml/h by a syringe pump (Ascor S.A., AP12). The electric potential applied between the tip of the needle and the grounded collector placed 15 cm below was equal to 30 kV. In order to produce uniaxially oriented fibers for magnetometric studies, we employed a collector consisting of two separated bars of a conductive material . The fibers were formed at 22 °C and humidity in the range from 30 to 40%. The last step to form ZnO was the NFs calcination in air, at 500 °C for 4 h.
Structural characterization of NFs was performed by X-ray diffraction (XRD) and transmission electron microscopy (TEM). A high-resolution powder diffractometer (Philips X’Pert MPD Pro Alpha1) employing CuKα1 radiation was used. The Bragg–Brentano geometry of the apparatus was modified by monochromatizing the incident beam using a Johansson Ge (111) monochromator. For detection, a linear semiconductor strip detector was used. The data were collected for 12 h. TEM and electron diffraction images were obtained on a JEM2000EX electron transmission microscope at an accelerating voltage of 200 kV.
Scanning electron microscopy (SEM) provided information on NFs morphology. SEM images were obtained on Hitachi SU-70 microscope at an accelerating voltage of 5 kV. Chemical composition was investigated by energy dispersive X-ray spectroscopy (EDX) with incident beam current 6.5 nA and accelerating voltage 15 kV (Thermo Scientific Ultra Dry). Light emission properties were probed by cathodoluminescence (CL) (Gatan MonoCl-3) with beam accelerating voltage of 15 keV and incident current of 6.5 nA. To gain general information about the magnetic properties, the Fe doped ZnO fibers were investigated using superconducting quantum interference device (SQUID) magnetometry at temperatures ranging from 2 K up to room temperature. Magnetic Force Microscopy (MFM) (Veeco, Nanoscope IIIa MultiMode with standard MESP-type tip) was applied to image the magnetic signal at room temperature. Prior to MFM the atomic force microscopy (AFM) in tapping mode (Nanoscope IIIa with OTESPA 160 μm tip) was used to check the vertical corrugations of the deposited fibers. MFM was performed in lift mode with lift height 150 nm, above the diameter of the thickest fibers.
3 Results and discussion
At temperatures below 50 K, we find that the magnetic signal does not saturate in magnetic fields below 10 kOe. It is a clear indication that a paramagnetic phase is also present in the NFs. This paramagnetic signal most likely originates from substitution Fe2+ and therefore demonstrates a formation of a (Zn,Fe)O ternary alloy.
We do not have all, direct or definitive evidence which mechanism is responsible for the observed ferromagnetism in our NFs. However we are inclined to the following two possibilities. The first one is related to Fe ions substitution in the ZnO matrix. These ions can form a robust ferromagnetic phase mediated by delocalized p-type carriers (holes)  or through a superexchange with oxygen vacancies . Since typically ZnO exhibits an n-type conductivity, we conclude that the latter mechanism is the more probable one. Indeed, recently the crucial role of oxygen vacancies in appearance of the ferromagnetic phase has been proved experimentally . We note that during the calcinations process the presence of carbon ions from precursor substances facilitate the formation of oxygen vacancies in our samples. The second possible explanation is related to a nanoscale phase separation responsible for the presence of Fe-rich magnetic nanoparticles . These particles can take form of α-Fe, various Fe-oxides and/or condensed (Zn, Fe) O. These particles can generate a strong ferromagnetic signal and remain not detected by our structural characterization methods.
In conclusion, we developed a fabrication method, which allows us to obtain nanofibers exhibiting ferromagnetism at room temperature. By electrospinning and calcination, we produce about 200 nm in diameter Fe doped ZnO fibers of virtually infinite length, build of about 4.5 nm crystallites oriented with 001 crystal axis perpendicular to the fiber axis. We demonstrate that some of the Fe atoms substitute Zn in the ZnO matrix and give rise to a paramagnetic signal at low temperatures. Incorporating 10% Fe ions does not modify the wurtzite crystal structure of the host ZnO. While the exact origin of the room temperature ferromagnetism remains unknown, we suggest that it is either due to a mechanism mediated by presence of oxygen vacancies or related to small precipitates of ferromagnetic phases of iron. Importantly, compared to previously reported Co and Mn doped ZnO based semiconductors, the synthesized material is a good candidate for biologically compatible therapeutic and diagnostic applications.
The research was partially supported by the European Union within European Regional Development Fund, through Grant Innovative Economy (POIG.01.01.02-00-008/08) and by the Ministry of Science and Higher Education (Poland) through Grant No. N518 424036 and No. N515 015 32/0997.
This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.
- 24.Baranowska-Korczyc A, Sikora B, Zaleszczyk W, Nowicka A, Fronc K, Wojciechowski T, Dziawa P, Knoff W, Gas K, Paszkowicz W, Szuszkiewicz W, Świątek K, Kłopotowski Ł, Sobczak K, Dłużewski P, Karczewski G, Wojtowicz T, Bujak J, Elbaum D (2009) ICFSI-12 in Weimar, abstract-book 302Google Scholar
- 30.Gopikrishnan R, Zhang K, Ravichandran P, Baluchamy S, Ramesh V, Biradar S, Ramesh P, Pradhan J, Hall JC, Pradhan AK, Ramesh GT (2010) Nano-Micro Lett 2(1):31–36Google Scholar
- 33.Data Base: JCPDS, file 36-1451Google Scholar